Long-range ordering during delithiation of LiMn2O4 cathode material
Björk, Helen; Gustafsson, Torbjörn; Thomas, John O.; Lidin, Sven; Petříček, Václav; Journal of Materials Chemistry 13 (2003) 585–; doi:10.1039/b210265j

data_7204553
_publ_section_title
;
 Long-range ordering during delithiation of LiMn2O4 cathode material
;
_journal_issue                   3
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              585
_journal_paper_doi               10.1039/b210265j
_journal_volume                  13
_journal_year                    2003
_chemical_formula_sum            'Li Mn2 O4'
_chemical_formula_weight         180.1
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.244(4)
_cell_length_b                   8.244(4)
_cell_length_c                   8.244(4)
_cell_measurement_radiation      'Mo K\a'
_cell_measurement_reflns_used    25
_cell_measurement_temperature    295
_cell_measurement_theta_max      20
_cell_measurement_theta_min      19
_cell_measurement_wavelength     0.71073
_cell_volume                     560.3(5)
_computing_cell_refinement       'STOE IPDS'
_computing_data_collection       'STOE IPDS'
_computing_data_reduction        'X-red and X-shape (STOE & Cie GmbH, 1996)'
_computing_molecular_graphics    -
_computing_publication_material  JANA2000
_computing_structure_refinement  DUPALS
_computing_structure_solution    -
_diffrn_ambient_temperature      295(2)
_diffrn_measurement_device       'Image plate diffractometer'
_diffrn_measurement_device_type  'STOE IPDS'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0568
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            1766
_diffrn_reflns_theta_max         40
_diffrn_reflns_theta_min         0
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  .
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    8.688
_exptl_absorpt_correction_T_max  0.377
_exptl_absorpt_correction_T_min  0.182
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.262
_exptl_crystal_description       octahedral
_exptl_crystal_F_000             680
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         0.67
_refine_diff_density_min         -0.77
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_obs   2.26
_refine_ls_goodness_of_fit_ref   2.03
_refine_ls_number_parameters     7
_refine_ls_number_reflns         108
_refine_ls_R_factor_all          0.0307
_refine_ls_R_factor_gt           0.0207
_refine_ls_shift/su_max          0.060
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w==1/(\s^2^(F)+0.000064F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0256
_refine_ls_wR_factor_ref         0.0262
_reflns_limit_h_max              14
_reflns_limit_h_min              1
_reflns_limit_k_max              10
_reflns_limit_k_min              0
_reflns_limit_l_max              8
_reflns_limit_l_min              0
_reflns_number_observed          85
_reflns_number_total             108
_reflns_observed_criterion       3\s
_cod_data_source_file            b210265j.txt
_cod_data_source_block           spinell
_cod_depositor_comments
;
The following automatic conversions were performed:
'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according to
'/home/adriana/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 

The following automatic conversions were performed:

'_diffrn_ambient_temperature' value 'ambient' was changed to '295(2)'
- the room/ambient temperature average [293;298] in Kelvins(K) was
taken.

Automatic conversion script
Id: cif_fix_values 1569 2011-02-09 13:29:24Z adriana 
;
_cod_original_cell_volume        560.5(5)
_cod_original_sg_symbol_H-M      Fd-3m
_cod_database_code               7204553